Effect of volume fraction of phases and precipitates on the mechanical
behavior of UNS S31803 duplex stainless steel
J.C. de Lacerdaa,b,⇑
, L.C. Cândidoa
, L.B. Godefroida aREDEMAT, Universidade Federal de Ouro Preto, 35400-000 Ouro Preto, MG, Brazil bUniversidade Federal de Itajubá – Campus Itabira, 35900-000 Itabira, MG, Brazil
a r t i c l e
i n f o
Received 22 June 2014
Received in revised form 26 December 2014 Accepted 27 December 2014
Available online 6 January 2015
Duplex stainless steel Microstructure Tensile and fatigue tests
a b s t r a c t
Mechanical properties of a grade UNS S31803 duplex stainless steel were studied. Samples were annealed at three different temperatures, 1060°C, 1200°C, and 1300°C, to change thea/cproportion, to
precipi-tate undesirable phases (for example,a0,rand chromium nitrides), and to study the effect of the micro-structure on the mechanical behavior. Specimens with a thickness of 1.8 mm were prepared according to ASTM standards and tested at room temperature. Tensile tests were conducted using displacement con-trol at a rate of 5 mm/min. Force-concon-trolled constant amplitude axial fatigue tests were conducted at a frequency of 30 Hz and anRstress ratio of 0.1. Microstructural analyses, performed by optical microscopy and scanning electron microscopy, showed the following modifications to the microstructure: changes in the phase volume fractions, the phase grain growths, and the morphology of thec-phase and the
precip-itation of chromium nitrides in thea-phase. The mechanical properties of the steel were significantly
changed due to the changed microstructure. The results demonstrate the sensitivity of the steel to the annealing temperature.
Ó2015 Elsevier Ltd. All rights reserved.
Duplex stainless steels are an important class of stainless steels
[1,2], with a dual-phase microstructure consisting of approxi-mately equal volume fractions of ferrite (
a) and austenite (
c). The balance between the two phases is obtained by means of heat treatment, whose temperature depends on the chemical composi-tion of the alloy. As a result of an interesting combinacomposi-tion between the austenitic and ferritic stainless steels, these duplex stainless steels combine the best features of both alloys, e.g., stress corrosion cracking resistance and good weldability and reduced costs due to the minor presence of alloying elements in comparison with other stainless steels[3–9]. Due to its low carbon content (i.e., less than 0.03%), duplex stainless steels are not susceptible to sensitization (i.e., chromium carbide precipitation in grain boundaries is virtu-ally eliminated), and therefore, they possess high resistance to intergranular corrosion. The addition of nitrogen to the duplex stainless steels increases the fracture toughness and the corrosion resistance of the heat-affected zone compared with welded base metal. With a low percentage of nickel in their chemical composi-tions, these steels exhibit a superior tensile yield stress than
austenitic stainless steels, enabling applications requiring thinner thicknesses and greater corrosion resistances.
An important grade of duplex stainless steels is the so-called ‘‘2205’’ (UNS S31803), which is used in the oil and gas industry in flexible pipes for oil extraction and in the pulp and paper indus-try in tanks for the storage of chemicals, products and equipment. Their mechanical resistance is promoted by a ferritic structure (interstitial solid solution, mainly N; substitutional solid solution, mainly Cr, Mo, Ni; grain refining, with mutual action between the phases), while the austenitic structure guarantees ductility and fracture toughness. Mixing phases also provides a good resis-tance to stress corrosion cracking and makes the alloy resistant to intergranular corrosion. Its high content of chromium and molybdenum is responsible for resistance against pitting corrosion and uniform corrosion[1,2].
One of the limitations with the use of duplex stainless steels is related to the thermal stability of the material; it is suggested to use only below 250–300°C. This is because of the large number
of undesirable precipitates formed in the
aphase at temperatures between 300 and 1000°C, such as
rand chromium nitrides. The elements Cr, Mo and W accelerate the precipitation and expand the range of the temperature. The main effect of the precip-itation is the embrittlement of the material and a decreased frac-ture toughness [9–24]. High temperatures can also change the
http://dx.doi.org/10.1016/j.ijfatigue.2014.12.015 0142-1123/Ó2015 Elsevier Ltd. All rights reserved.
⇑ Corresponding author at: Universidade Federal de Itajubá – Campus Itabira, 35900-000 Itabira, MG, Brazil. Tel.: +55 31 38390848.
E-mail address:email@example.com(J.C. de Lacerda).
Contents lists available atScienceDirect
International Journal of Fatigue
amount, morphology and distribution of phases, and this may cause loss of toughness and corrosion resistance.
This work studied the tensile and fatigue (i.e., load control) strengths of a UNS S31803 duplex stainless steel. Samples were annealed at three different temperatures to verify thermal effects on the mechanical properties of the material. The temperatures were chosen to cause a change in the volume fraction of
cphases and the possible precipitation of undesirable phases. These heat treatments were chosen to simulate any high temperature applica-tions of the steel in or any welding procedure found during the fab-rication of an engineering structure.
2. Experimental procedures
The steel studied was supplied by APERAM South America, Timóteo city, Minas Gerais state, Brazil, in the form of cold-rolled sheets. Its nominal chemical composition is presented inTable 1. Rectangular cross-sections and continuous radius between ends 1.8 mm thick specimens were prepared according to specific ASTM standards[25,26]. The specimens were removed in the longitudi-nal section of rolling direction, and annealed at three tempera-tures: 1060°C, 1200°C and 1300°C. Fig. 1 shows the curves of
heating and cooling applied for the annealing treatments. The mechanical tests were performed on a servo-hydraulic MTS machine at room temperature. Tensile tests were performed with displacement control at a rate of 5 mm/min. The fatigue tests were conducted with load control, at a frequency of 30 Hz and anRratio of 0.1. In all mechanical tests, three specimens were used for each situation. Microstructure samples taken from a section longitudi-nal to the rolling direction were examined on a Leica optical micro-scope and a JEOL scanning electron micromicro-scope.
cphases were treated and exposed with a reagent consisting of 1 g of K2S2O5in 15 ml of HCl diluted in 85 ml of distilled water, with an exposure time of 5 s[20,27]. Precipitates were collected using an electrolyte solution consisting of oxalic acid solution (10%) at 5 V and 15 s[15–17]. The fracture image analysis was conducted using a JEOL scanning electron microscope.
3. Results and discussion
Fig. 2presents the microstructure of the steel after annealing at the three temperatures. At 1060°C, it is possible to see a fibrous
Chemical composition of the steel studied (wt%).
C Cr Ni Mo N Si Mn V Co Sn Ti Nb Cu W
0.02 22.38 5.35 3.04 0.151 0.31 1.82 0.06 0.02 0.01 0.01 0.04 0.2 0.01
0 100 200 300 400 500 600 0
200 400 600 800 1000 1200 1400
T = 1060°C T = 1200°C T = 1300°C
Fig. 1.Heat treatments applied to the UNS S31803 stainless steel.
microstructure, typical of the rolling process. The austenitic phase appears as islands with a light tone, and the ferritic phase is the matrix that surrounds the austenitic phase and is present in a darker tone. At 1200°C, the heat treatment leads to a strong
recrystallization and grain coarsening of both phases. At 1300°C,
a different morphology is observed, with a larger ferrite grain size, Table 2
Volume fraction ofa/cphases for different annealing temperatures.
T(°C) 1060 1200 1300
aPhase 51 ± 2 62 ± 4 74 ± 3
cPhase 49 ± 2 38 ± 4 26 ± 3
Fig. 3.Variation of volume fraction of phases for different annealing temperatures.
Fig. 4.Presence of chromium nitride precipitates in the duplex stainless steel (circle) after heat treatment atT= 1300°C. SEM image.
Fig. 5.Variation of phase hardness for different annealing temperatures.
Fig. 6.Tensile stress–strain curves for different annealing temperatures.
Fig. 7.Tensile mechanical resistance for different annealing temperatures.
Fig. 8.Tensile strain to fracture for different annealing temperatures.
and acicular grains of austenite located on the boundaries of the ferrite grains. Annealing also changed the volume fractions of the present phases.Table 2shows the ferritic phase fraction increasing with the annealing temperature.Fig. 3shows that the dependence of the phase volume fractions on the annealing temperature fol-lows a linear trend. The effect of annealing temperature on the fer-ritic grain size can be seen inTable 3. All results are in accordance with previously reported data in the literature.
The chemical etching revealed the presence of chromium nitrides in the material annealed at 1300°C, precipitated in ferrite
grains, as reported by other researchers studying duplex stainless steels with similar volume fractions of ferrite [4,20,28]. Fig. 5
shows fine distributions of these precipitate clusters inside the fer-rite grains. The precipitation of chromium nitrides in the steel annealed at 1300°C was due to the low solubility of nitrogen in
the ferrite and an increase in volume fraction of this phase, approx-imately 74%, relative to the austenite fraction. It is interesting to note the absence of
rphase in the microstructure of steel trea-ted at 1300°C. This is due to the high cooling rate imposed on the
material between 1000 and 600°C (20°C/s, seeFig. 1), which
pre-vents the formation of this phase.
Table 4 andFig. 5 show the hardness variation (i.e., Vickers microhardness) of the
cphases as a function of the annealing temperature. It is possible to see a significant increase in the hard-ness of the ferrite phase, confirming the precipitation of chromium nitrides at 1300°C (Fig. 4), even with an increase in the ferritic
grain size (Table 3).
Fig. 6shows the engineering stress–strain curves obtained in the tensile tests as a function of the annealing temperatures. The
Fig. 9.Fractography of tensile specimens. SEM images.
Fig. 10.Maximum stress and fatigue life for different annealing temperatures.
main mechanical properties obtained from these curves are pre-sented inTable 5.Figs. 7 and 8show trend curves for the relation-ships between the mechanical properties and the annealing
temperature. A decrease in the mechanical strength is observed for an increasing annealing temperature, due to the increase of grain sizes and changes in the volume fractions and the Fig. 12.Fractography of fatigued specimens, start and intermediate regions of cracking. Dashed arrows indicate the direction of crack growth. SEM images.
morphologies of the two phases. As the total deformation (and consequently, the fracture toughness) decreases with increasing temperature, it is assumed that the presence of chromium nitrides precipitates also contributes to these results[10–12]despite the tendency for embrittling ferrite (i.e., an observed hardness increase, seeTable 4andFig. 5).
Regardless of the influence of the annealing temperature on the tensile mechanical properties of duplex stainless steels, the frac-ture had a ductile nafrac-ture and developed by a mechanism of nucle-ation, growth and coalescence indicative of microvoids formation
.Fig. 9illustrates this mechanism for the three studied temper-atures. The only difference between the samples is the dimple size, which grows with increasing annealing temperature. The dimple size is correlated with the increase in the grain size of both phases (seeTable 3). It is interesting to note that the presence of hardener precipitates in the ferritic phase of the steel treated at 1300°C did
not change the mechanism of the tensile fracture.
Fig. 10presents the results obtained in the fatigue tests with load controls, in the form of curves of maximum stress versus the number of cycles to fracture. Exponentially decaying trend curves were fit to better interpret the data and to facilitate a com-parison between the three distinct situations. The chart is divided into three regions according to the different behaviors for the fati-gued material: low cycle fatigue (i.e., where the maximum stress exceeds the tensile yield stress), high cycle fatigue (i.e., where the maximum stress is below the tensile yield stress), and ‘‘infinite life’’ (i.e., samples that did not fracture after 107cycles). In this last region, the points shown in the figure correspond to the 5 speci-mens that did not fracture. Increasing the annealing temperature negatively impacts the fatigue performance of the steel, particu-larly the low cycle behavior and the fatigue limit. The wide disper-sion of results in the high cycle fatigue region prevented a verification of the steel performance.Fig. 11shows the traditional relationshipbetween the ultimate tensile stress and the fati-gue limit for the steel studied at the three temperatures.
The study of fatigue resistance in duplex stainless steels has interested several researchers over the last two decades[30–54]. There is a consensus that the fatigue crack nucleation is heavily dependent on characteristics of both phases, such as the volume fraction, morphology, cyclic hardening/softening, crystallographic orientation, activation of slip bands and twinning, and brittle phase precipitation on ferrite. There is also a consensus that fatigue cracking mechanisms depend on the stress/strain level in the material (i.e., low/high fatigue cycle) and that interfaces between phases play an important role in the crack growth resistance. In this study, the ferrite hardness increased with increasing annealing temperature (due to chromium nitrides precipitates; see Figs. 4 and 5) and transferred the plastic deformation to the austenite phase, where fatigue crack nucleation is more probable. Once nucleated in the austenite phase, cracks readily propagated in the more brittle ferrite. The morphology change of austenite grains and the decrease of
cinterfaces with increasing temperature helped to decrease the growth resistance of these cracks. In this way, the degradation of fatigue resistance with increasing temper-ature was verified.
Fractographic analysis also revealed important features about the effect of annealing temperature on fatigue cracking. To facili-tate the comparison between the three distinct situations, speci-mens that broke after approximately 106cycles (i.e., close to the fatigue limit region) were chosen for each steel. Regardless of the sample treatment condition, fatigue cracking initiated on the sur-face of the specimen, in a region near a corner (i.e., a stress concen-trator site). In all specimens, it was possible to identify the initial nucleation region where fatigue cracking began, the intermediate region of active fatigue cracking and the final tearing region. The nucleation region showed a predominantly transgranular fracture
mode, with a ‘‘hill-and-valley’’ type appearance, shear facets, and an associated zig-zag crack path. Such fractures show high rough-ness and crack deflection angles. At higher growth rates, fracture surfaces remain transgranular but with evidence of striations. In the tearing region, tensile stresses cause the same ductile behavior as shown in the tensile tests. These characteristics are shown inFig. 12(a–f).
In the region of the fatigue crack nucleation, shear planes with a greater slipping surface area were observed in steel treated at 1300°C. This morphology is due to the larger grain size and
soften-ing of the
cphase present in that steel (Tables 3 and 4). In the intermediate/final region of the fatigue cracking, the steel treated at 1300°C presented thicker striations. This morphology indicates
a higher crack growth rate (Fig. 10) and is primarily due to the hardening ferritic phase (Table 4). These fractographic characteris-tics confirm the deleterious effect of the presence of chromium nitride precipitates in the ferrite grains.
An investigation of the effects of annealing at 1060°C, 1200°C
and 1300°C on the microstructure and mechanical properties of
a UNS S31803 duplex stainless steel reached the following conclusions:
The increase in temperature caused a significant change in the microstructure of the steel, with changes in the volume fraction and the morphology of the ferrite and austenite phases, increases in the grain size of both phases, and the precipitation of chromium nitrides in the ferrite;
these microstructural changes resulted in a decreased tensile mechanical strength and ductility of the steel due to the increase in grain size of the two phases, an increase in the vol-ume fraction of ferrite and the presence of chromium nitride precipitates in the ferrite;
these microstructural changes also caused a decrease in the fati-gue crack resistance;
the nucleation of fatigue cracks was facilitated in the austenitic phase with an increasing annealing temperature due to the transfer of the plastic deformation of the ferritic phase (hard-ened by the presence of precipitates) to the austenitic phase; Table 3
ASTM ferritic and austenitic grain size for different annealing temperatures.
T(°C) 1060 1200 1300
Ferrite 16.3 13.5 10.5
Austenite 16.4 14.9 11.7
Vickers microhardness of thea/cphases for different annealing temperatures.
T(°C) 1060 1200 1300
aPhase 289 ± 14 283 ± 12 347 ± 15
cPhase 365 ± 16 341 ± 19 315 ± 13
Tensile mechanical properties for different annealing temperatures.rYS: yield stress; rUTS: ultimate tensile stress;e: total strain.
T(°C) 1060 1200 1300
rYS(MPa) 650 ± 4 626 ± 10 632 ± 11
rUTS(MPa) 818 ± 10 789 ± 2 763 ± 20
the growth of fatigue cracks was facilitated in the ferritic phase with an increasing annealing temperature due to the hardening of their grains (due to the presence of precipitates), and the reduction of
cinterfaces with a grain coarsening of both phases; and
all the results demonstrate the sensitivity of the steel to the annealing temperature and the care that must be taken in using this steel in applications with large variations in temperature.
The authors acknowledge Ricardo A. Faria, Ph.D. from APERAM South America for the supplied specimens.
 Soluções sustentáveis em aço inoxidável para toda a cadeia de óleo e gás. APERAM South America;www.aperam.com(accessed 3.04.2013).
 Charles J, Faria RA. Aços inoxidáveis duplex e aplicações em óleo e gás;www. nucleoinox.org.br/upfiles/arquivos/downloads/inox08/pg_247-254.pdf (accessed 03.04.2013).
Davis JR. Stainless steels handbook. The Materials Information Society (ASM); 1996.
Pohl M, Storz O, Glogowski T. Effect of intermetallic precipitations on the properties of duplex stainless steel. Mater Charact 2007;58:65–71. Neessen F, Bandsma P, Smitweld L. Tankers – a composition in duplex stainless
steels. Weld Innov 2001;18:3–8.
Horvarth W, Prantl W, Stuwe HP, Werner E. Influence of thermal cycling on the microstructure of a ferritic–austenitic duplex stainless steel. Mater Charact 1995;34:277–85.
Olsson J, Snis M. Duplex – a new generation of stainless steels for desalination plants. Desalination 2005;205:104–13.
Hussain EAM, Robinson MJ. Erosion–corrosion of 2205 duplex stainless steel in flowing seawater containing sand particles. Corros Sci 2007;49:1737–54.  IMOA (International Molybdenum Association). Practical Guidelines for the
Fabrication of Duplex Stainless Steel, 2nd ed. London; 2009. 64 page.  Moreno JRS. Degradação da resistência à corrosão de aços inoxidáveis duplex
devido ao envelhecimento em baixas temperaturas por tempos prolongados. Thesis. UFSCar, Brazil; 2004. 196 page.
 Pinto TB. Comportamento mecânico de um aço inoxidável duplex do tipo 2205 sob a influência da temperatura e da precipitação de fases frágeis. Thesis. Unicamp, Brazil, 2001. 214 page.
 Fontes TF. Efeito da fasea0nas propriedades mecânicas e de resistência à corrosão do aço inoxidável duplex UR 52N+. Dissertation. IPEN, Brazil; 2009. 93 page.
Michalska J, Sozanska M. Qualitative and quantitative analysis ofrandv
phases in 2205 duplex stainless steel. Mater Charact 2005;56:355–62. Sieurin H, Sandström R. Sigma phase precipitation in duplex stainless steel
2205. Mater Sci Eng, A 2007;444:271–6.
Magnabosco R. Kinetics of sigma phase formation in a duplex stainless steel. Mater Res 2009;12(3):321–7.
 Magnabosco R, Bruno D. Efeito do envelhecimento a 475 C na microestrutura e corrosão por pite do aço inoxidável dúplex UNS S31803 (SAF 2205). In: 62 Congresso Internacional Anual da ABM, Vitória, Brazil; 2007.
Nascimento AM, Sampaio JP, Machado E, Sobral AVC, Abreu HFG. Estudo das transformações de fase do aço inoxidável duplex UNS S31803 quando submetido a altas temperaturas. Revista Tecnologia 2003;24:13–22. Fortaleza, Brazil.
Badji R, Bouabdallah M, Bacroix B, Kahloun C, Belkessa B, Maza H. Phase tansformation and mechanical behavior in annealed 2205 duplex stainless steel welds. Mater Charact 2008;59:447–53.
Zucato I, Moreira MC, Machado IF, Lebrão SMG. Microstructural characterization and the effect of phase transformations on toughness of the UNS S31803 duplex stainless steel age treated at 850°C. Mater Res 2002;5:385–9.
Fargas G, Anglada M, Mateo A. Effect of the annealing temperature on the mechanical properties, formability and corrosion resistance of hot-rolled duplex stainless steel. J Mater Process Technol 2009;209:1770–82. Weng KL, Chen HR, Yang JR. The low-temperature aging embrittlement in a
2205 duplex stainless steel. Mater Sci Eng 2004;A379:119–32.
Hättestrand M, Larsson P, Chai G, Nilsson JO, Odqvist J. Study of decomposition of ferrite in a duplex stainless steel cold worked and aged at 450–500°C. Mater Sci Eng 2009;A499:489–92.
Silva EM, Albuquerque VHC, Leite JP, Varela ACG, Moura EP, Tavares JMRS. Phase transformations evaluation on a UNS S31803 duplex stainless steel based on non-destructive testing. Mater Sci Eng 2009;A515:126–30. Chandra K, Singhal R, Kain V, Raja VS. Low-temperature embrittlement of
duplex stainless steel: correlation between mechanical and electrochemical behavior. Mater Sci Eng 2010;A527:3904–12.
 ASTM E8M. Standard Test Methods for Tension Testing of Metallic Materials.  ASTM E466-07. Standard Practice for Conducting Force Controlled Constant
Amplitude Axial Fatigue Tests of Metallic Materials.
 Reis TJA, Andrade MS, Godefroid LB. Efeito de tratamentos isotérmicos a 475 C e a 850 C na resistência à fadiga de um aço inoxidável duplex UNS S32304. In: 68 Congresso Internacional Anual da ABM, Belo Horizonte, Brazil; 2012. Tavares SSM, Terra VF, Pardal MP, Cindra Fonseca MP. Influence of the
microstructure on the toughness of a duplex stainless steel UNS S31803. J Mater Sci 2005;40:145–54.
Godefroid LB, Cândido LC, Morais WA. Análise de Falhas. Brazil: Associação Brasileira de Metalurgia, Materiais e Mineração – ABM; 2012.
 Llanes L, Mateo A, Anglada M. Cyclic response of duplex stainless steel – an intrinsic two-phase description. In: Proceedings of the Sixth International Fatigue Conference. Berlin/Germany, Pergamon; 1996. p. 87–92.
 Mateo A, Violan P, Llanes L, Mendez J, Anglada M. Fatigue life of duplex stainless steel – influence of ageing and environment. In: Proceedings of the Sixth International Fatigue Conference. Berlin/Germany, Pergamon; 1996. p. 209–214.
 Chai G, Sundqvist M. Fatigue strength and crack behavior of duplex stainless steel. In: Proceedings of the Seventh International Fatigue Conference. Beijing/ China, EMAS, 1999. p. 175–180.
 Baffie N, Gironès A, Mateo A, Anglada M, Stolarz J. Influence of interfaces on LCF short crack propagation in the bulk in single phase and in duplex stainless steels. In: Proceedings of the Seventh International Fatigue Conference. Beijing/China, EMAS, 1999. p. 359–364.
Mateo A, Llanes L, Akdut N, Anglada M. High cycle fatigue behaviour of a standard duplex stainless steel plate and bar. Mater Sci Eng, A 2001;319– 321:516–20.
Bugat S, Besson J, Gourgues AS, N’Guyen F, Pineau A. Microstructure and damage initiation in duplex stainless steels. Mater Sci Eng, A 2001;317:32–6. Vogt JB, Massol K, Foct J. Role of microstructure on fatigue properties of 475 C
aged duplex stainless steel. Int J Fatigue 2002;24:627–33.
 Mateo A, Gironès A, Llanes L, Anglada, M. Cyclic deformation and fatigue behavior of duplex stainless steel. In: Proceedings of the Eighth International Fatigue Conference. Stockholm/Sweden, EMAS; 2002. p. 461–472.
 Stolarz J, Baffie N. Low cycle fatigue of aged duplex steels. In: Proceedings of the Eighth International Fatigue Conference. Stockholm/Sweden, EMAS; 2002. p. 2831–2838.
Mateo A, Llanes L, Akdut N, Stolarz J, Anglada M. Anisotropy effects on the fatigue behaviour of rolled duplex stainless steels. Int J Fatigue 2003;25:481–8.
 Gironès A, Villechaise P, Mateo A, Anglada M, Méndez J. EBSD studies on the influence of texture on the surface damage mechanisms developed in cyclically loaded aged duplex stainless steels. Mater Sci Eng, A 2004;387– 389:516–21.
Chai G. Fatigue behavior of duplex stainless steels in the very high cycle regime. Int J Fatigue 2006;28:1611–7.
 Düber O, Künkler B, Krupp U, Christ HJ, Fritzen CP. Short crack propagation in duplex stainless steel. In: Proceedings of the Ninth International Fatigue Conference. Atlanta/USA, Elsevier; 2006, CD_ROM.
Alvarez-Armas I, Marinelli MC, Malarría JA, Degallaix S, Armas AF. Microstructure associated with crack initiation during low-cycle fatigue in a low nitrogen duplex stainless steel. Int J Fatigue 2007;29:758–64.
Armas AF, Hereñú S, Alvares-Armas I, Degallaix S, Condó A, Lovely F. The influence of temperature on the cyclic behavior of aged and unaged super duplex stainless steels. Mater Sci Eng, A 2008;491:434–9.
El Bartali A, Aubin V, Sabatier L, Villechaise P, Degallaix S. Identification and analysis of slip systems activated during low-cycle fatigue in a duplex stainless steel. Scripta Mater 2008;59:1231–4.
Balbi M, Avalos M, El Bartali A, Alvarez-Armas I. Microcrack growth and fatigue behavior of a duplex stainless steel. Int J Fatigue 2009;31:2006–13. El Bartali A, Aubin V, Degallaix S. Surface observation and measurement
techniques to study the fatigue damage micromechanisms in a duplex stainless steel. Int J Fatigue 2009;31:2049–55.
Marinelli MC, El Bartali A, Signorelli JW, Evrard P, Aubin V, Armas IA, et al. Activated slip systems and microcrack path in LCF of a duplex stainless steel. Mater Sci Eng, A 2009;509:81–8.
Sahu JK, Gosh RN, Christ HJ. Low cycle fatigue behavior of duplex stainless steel – influence of isothermal aging treatment. Fatigue Fract Eng Mater Struct 2009;33:77–86.
 Christ HJ, Düber O, Fritzen CP, Knobbe H, Köster P, Krupp U, et al. Propagation behaviour of microstructural short fatigue cracks in the high-cycle fatigue regime. Comput Mater Sci 2009;46:561–5.
Alvares-Armas I, Knobbe H, Marinelli MC, Balbi M, Hereñú S, Krupp U. Experimental characterization of short fatigue crack kinetics in an austeno-ferritic duplex steel. Proc Eng 2011;10:1491–6.
Sahu JK, Krupp U, Christ H. Fatigue crack initiation behavior in embrittled austenitic–ferritic stainless steel. Int J Fatigue 2012;45:08–14.
Strubbia R, Hereñú S, Marinelli MC, Alvares-Armas I. Short crack nucleation and growth in lean duplex stainless steel fatigue at room temperature. Int J Fatigue 2012;41:90–4.
Alvares-Armas I, Krupp U, Balbi M, Hereñú S, Marinelli MC, Knobbe H. Growth of short cracks during low and high cycle fatigue in a duplex stainless steel. Int J Fatigue 2012;41:95–100.